Electrochemical and Solid-State Letters, 10 共7兲 A166-A170 共2007兲 A166 1099-0062/2007/10共7兲/A166/5/$20.00 © The Electrochemical Society Enhanced Low-Temperature Performance of Li–CFx Batteries J. F. Whitacre,a,*,z W. C. West,a,* M. C. Smart,a,* R. Yazami,b,* G. K. Surya Prakash,c,* A. Hamwi,d and B. V. Ratnakumara,* a Jet Propulsion Laboratory, California Institute of Technology, Pasadena, California, USA California Institute of Technology, Pasadena, California, USA c University of Southern California, Los Angeles, California, USA d Université Blaise Pascal de Clermont-Ferrand, 63177 Aubière, France b This work describes the continued examination of the low-temperature performance of the Li–CFx electrochemical couple in a −40°C or colder environment. Previously, the efficacy of subfluorinated CFx 共SFCFx兲 cathode active materials was demonstrated; preliminary results indicated that the material was functional at rates up to C/10 at −40°C. However, there were often substantial voltage fluctuations during discharge, accompanied with inconsistent capacity yields and sometimes dramatic polarization events. In the research described herein, an investigation of various electrolyte and cathode compositions was conducted in an effort to optimize performance. In particular, several different electrolyte solvent formulations were examined using a salt content of either 1 or 0.5 M LiBF4. A further modification consisted of addition of an anion receptor to the electrolyte that was intended to be a LiF-solvating agent. The most promising electrolyte was tested with several different SFCFx compositions created using either graphitic or multiwall nanotube precursor materials. Electrochemical evaluation showed that the best SFCFx-based test cells were able to deliver specific capacity values up to five times greater than control cells 共containing conventional CF1.08 powder兲 at −40°C under discharge currents as high as C/5 with composite electrodes thicker than 100 m. © 2007 The Electrochemical Society. 关DOI: 10.1149/1.2735823兴 All rights reserved. Manuscript submitted December 20, 2006; revised manuscript received March 8, 2007. Available electronically May 3, 2007. Recently, it has been reported that subfluorinated CFx 共SFCFx兲 materials 共where 0.3 ⬍ x ⬍ 0.66兲 are capable of supporting discharge rates as high as 5C at room temperature with excellent utilization.1 It was unknown, however, whether these cathodes would possess the same characteristics at very low temperatures at aggressive rates 共i.e., greater than C/100兲. The significantly slower cathode reaction kinetics and/or lower electrolyte ionic conductivity values at these temperatures could mitigate the benefits observed at room temperature. Furthermore, the factors that cause the voltage delay effect in Li–共CF兲n batteries are likely to be more prominent under high-rate, low-temperature conditions and therefore must be examined if a functional battery is to be eventually produced. Preliminary results have been published recently,2 where it was indicated that the subfluorinated CFx materials did exhibit superior lowtemperature performance at −40°C compared to baseline CF1, though at current levels not exceeding a C/20 rate. Two electrolyte blends were compared: 1 M LiBF4 solvated in a DME/PC mix to a ratio of either 80:20 or 50:50 v/v %. The 80:20 v/v % 1, 2-dimethoxyethane 共DME兲/propylene carbonate 共PC兲-based electrolyte had superior performance at low temperatures, though there were still significant variations in cell performance at higher rates at −40°C.2 It was unclear whether this erratic behavior was due to the inherent properties of the electrolyte, interfacial properties 共i.e., cathode surface wettability兲, or the redistribution of reaction byproducts 共LiF兲 upon discharge. The focus of the work presented in this letter is to further improve low-temperature functionality by matching the highest capacity subfluorinated cathode active material with the proper electrolyte blend and electrode form factor. In particular, three different electrolytes were tested at low temperatures with a standard Li–CF0.65 cell. The best electrolyte was then used to test several variations of subfluorinated CFx cathode material. These results were compared to those obtained from cathodes produced using commercially available CF1.08. In some cells, a solvating anion receptor additive was also inserted into the electrolyte with the intention of reducing cathode surface Li–F passivation, thereby increasing the electrode functionality. The most promising test cells were able to support substantial discharge currents at temperatures colder than −40°C, with composite cathode thicknesses exceeding 110 m. * Electrochemical Society Active Member. z E-mail: [email protected] Experimental A standard test vehicle was adopted that consisted of a spraydeposited cathode layer containing 10% poly共vinylidene difluoride兲 共PVDF兲 binder, 10% carbon black, and 80% active material on a 1 mil thick Al current collector foil heated. These composite cathodes ranged in thickness from 10 to 120 m, with the most commonly tested thickness being about 40 ± 5 m. The relationship between electrode mass and thickness was determined using a precision caliper on the thicker samples 共⬎50 m兲. The standard test cell consisted of 2032 coin cells with a Li metal anode and a single layer of polypropylene 共Tonen兲 separator. The control electrode, based on CF1.08 as received from a commercial vendor, contained 30 wt % carbon black and 10 wt % PVDF. This resulted in a composite electrode capable of similar room-temperature performance 共per unit mass of the total composite electrode兲 as a CF0.55-containing electrode.2 A representative SFCFx electrode composition and thickness, CF0.65 and 40 ± 5 m thick, was first used to identify promising electrolyte blends for low-temperature performance. The selected electrolyte blends are indicated in Table I. The lithium tetrafluoroborate used was battery grade obtained from Mitsubishi Petrochemicals Co. and was vacuum dried prior to use. The PC and DME were also high-purity battery grade and obtained from Mitsubishi Petrochemicals Co. and were used as received. The trifluoroethyl ether 共TEE兲 and trifluoropropylene carbonate 共TFPC兲 were synthesized at the University of Southern California by a known method consisting of the acid-catalyzed dehydration reaction of 2,2,2-trifluoroethanol. The rationale for incorporating ethers bearing fluoroalkyl groups in electrolyte formulations is twofold: 共i兲 they are envisioned to Table I. Electrolyte solvent/salt blends initially tested for lowtemperature efficacy in the Li/CFx test cells. The performance of 1 M M LiBF4 solvated in 50:50 v/v % PC/DME at low temperatures is published elsewhere.2 Solvent 共v/v %兲 Salt PC/DME 共2:8兲 PC/TEE/DME 共2:2:6兲 PC/DME 共2:8兲 PC/TFPC/DME 共15:5:80兲 VC 共1.5兲 added to DME/PC 共2:8兲 1 M LiBF4 1 M LiBF4 0.5 M LiBF4 1 M LiBF4 1 M LiBF4 Electrochemical and Solid-State Letters, 10 共7兲 A166-A170 共2007兲 A167 Figure 1. 共Color online兲 Discharge data from Li–CF0.65 test cells at −40°C at a C/10 rate. All electrodes were 40 ± 5 m in thickness. Five different electrolytes are compared here. The two cells that offered very little capacity at this discharge rate were then subsequently discharged at a C/40 rate and yielded full capacity 共500 mAh/g above 1.5 V兲. impart beneficial physical properties to the electrolyte, due to their low viscosity, low melting points, and good solvating properties, and 共ii兲 the hydrofluorocarbon ethers are anticipated to better wet the CFx electrode, improving the interfacial properties. The optimization of the PC+DME blends is based upon the balance of having an adequate proportion of the high dielectric constant component 共PC兲 and a sufficient proportion of the low-viscosity, good coordinating component 共DME兲. During the course of optimization of these electrolytes for low-temperature operation, higher conductivity is observed with electrolyte formulations containing low PC content and low electrolyte salt concentration. In addition to these factors, the primary solvent, propylene carbonate or PC, needs to be in adequate proportion to impart passivation to the anode 共and hence shelf life to the cell兲 but not high enough to contribute to higher viscosity at low temperatures. Upon determining the highest performing electrolyte, at low temperatures, of those examined, test cells were made and tested using four different cathode active materials; three were SFCFx-based, and the last was the CF1.08-based standard. The SFCFx fabrication process is described elsewhere.3 The CF0.65 electrodes used partially fluorinated Madagascar graphite precursor, while the other two SFCFx variations contained CF0.59 or CF0.82 material made using multiwall carbon nanotube material precursor materials supplied by MER Corporation 共Tucson, AZ兲. Characterization data indicated that all of the SF CFx materials were comprised of pristine unfluorinated graphite domains mixed intimately with nanodispersed near-fully fluorinated graphitic regions and are consistent with data reported previously.1-3 The small scale of these regions dictates that the materials had a very high graphite-to-CF surface area and subsequently might possess excellent electronic/interfacial transport properties. In several of the 0.5 M LiBF4 in DME/PC 共80:20兲 containing cells, an anion receptor Lewis acid additive, tris共2,2,2-trifluoroethyl兲 borate 共TTFEB兲, was also dissolved into the electrolyte solvent in an effort to decrease or eliminate the LiF 共discharge reactant兲 electrode surface buildup via a F− complexing reaction. Such an approach has been employed elsewhere, with a variety of anion receptor molecules in Li-ion battery electrolytes, mainly to enhance the solubility of lithium salts.4-6 The nominal TTFEB concentration in the electrolyte solution was 1.5:98 v/v % TTFEB/共DME/PC兲 共80:20兲. Previous work indicated that a room-temperature predischarge step 共consisting of a 1 h, discharge at a C/33 current level兲 was necessary to prepare the electrode interfacial regions to accommodate low-temperature discharge.2 This preparation was used here for most test cells; however, the necessity of this predischarge was reexamined for the most promising electrode/electrolyte combinations. In all cases, the C rate was calculated based on the expected room-temperature capacity of the cathode if discharged at a C/40 rate. Results Figure 1 shows discharge data from CF0.64 SFCFx active-material cells using a C/10 discharge rate at −40°C with the different electrolytes listed in Table I. The best 共highest power, smoothest discharge curve兲 result was obtained with 0.5 M LiBF4 solvated in an 8:2 v/v % DME/PC blend. Test cells made with electrolytes that had a higher salt content 共1 M兲, were more rate-limited and had erratic potential variations during discharge at these low temperatures. Repeated testing supports this finding. Those cells that polarized rapidly were still functional and displayed smooth discharge curves and good discharge capacities at lower rates 共C/20 or slower兲 at −40°C. The execution of the predischarge step in the 0.5 M salt content cells was found to have no beneficial effect on low-temperature performance, in contrast to the results obtained using electrolytes containing higher salt concentrations. Electrical impedence spectroscopy 共EIS兲 data collected from test coin cells with stainless steel blocking electrodes indicate that the 1 M salt-content electrolyte had approximately twice the high-frequency, real-axis intercept at −40°C compared to the 0.5 M salt-containing blend. Figure 2 shows EIS data from Li/CF0.64 cells with either a 1 or 0.5 M salt content. Figure 2c contains the same data for a 0.5 M salt-content cell with the anion-receptor additive. All of these cells had similar active material masses and similar impedance characteristics after discharge. Figure 3 shows a comparison between the −40°C temperature performances of various CFx cathodes 共of similar mass/thickness兲 as discharged at the C/5 rate using the 0.5 M LiBF4 solvated in 8:2 v/v % DME/PC electrolyte. The thickness of the CF1.08-based cathode was 35 m, while the thickness of the SFCFx cathodes was A168 Electrochemical and Solid-State Letters, 10 共7兲 A166-A170 共2007兲 Figure 3. 共Color online兲 Discharge data from various Li–CFx test cells at −40 °C at a C/5 rate. All cells were 40 ± 5 m in thickness. The cells containing SFCFx yielded significantly more capacity at higher discharge potentials than that for the cell containing commercially available CF1.08. The highest capacity material was CF0.82 共multiwalled nanotube, MWNT, precursor兲, which delivered over 650 mAh/g above 1.5 V. The open squares are data from the thickest of the SFCFX electrodes 共57 m兲. the CF1.08 baseline cathode under identical discharge conditions. Multiple electrodes were tested for each electrode composition with consistent results. The composite cathode thickness has previously been found to have a strong negative correlation with the maximum usable discharge rate or realized discharge capacity in the Li–CFx chemistry and was therefore examined here under low-temperature conditions.7,8 Figure 4 shows the behavior of CF0.65 composite cathodes with thicknesses varying from 4 to 118 m at a C/5 discharge Figure 2. 共Color online兲 EIS data collected from Li–CF0.65 cells before and after full discharge at −40°C with 8:2 v/v % DME/PC electrolyte solvent using 共a兲 1 M LiBF4, 共b兲 0.5 M LiBF4, and 共c兲 0.5 M LiBF4 with anion receptor. The frequency range was 100,000 Hz to 50 mHz, while the cells were held at open-circuit potentials as measured after 30 min of equlibration. 40–60 m. The delivered capacities for the SFCFx cathodes were as much as 300% greater with the subfluorinated cathodes than that of Figure 4. 共Color online兲 Discharge behavior at a C/5 rate, −40°C as a function of composite cathode thickness, for CF0.65-based test cells. The 0.5 M LiBF4 with 8:2 v/v % DME/PC electrolyte was used in all cases, and the TTFEB anion acceptor was added in the thick electrode case 共115 m thick兲. Electrochemical and Solid-State Letters, 10 共7兲 A166-A170 共2007兲 Figure 5. 共Color online兲 High-rate, low-temperature performance of LiCF0.65 cells with anion receptor added to the 0.5 M LiBF4 with 8:2 v/v % DME/PC electrolyte. At −60°C, over 250 mAh/g was delivered at a C/5 rate. The composite cathode structures were approximately 40 m thick for these tests. rate. The cells delivered nearly full capacity, with some polarization and voltage delay, up to a thickness of at least 57 m. Cathodes as thick as 95 m or higher were severely polarized upon discharge under these conditions but were able to deliver full capacity at reduced discharge rates, for example at a C/10 rate for the 95 m cathode and at a C/40 rate for the 118 m thick cathode 共these results are not shown兲. The use of the TTFEB anion-receptor additive resulted in even thicker composite electrodes that could be made functional at these temperatures. Figure 4 also contains the results from a 115 m thick CF0.65 cathode discharged at a C/5 rate at −40°C with the anionreceptor additive. Figure 5 contains plots of Li–CF0.65 cells made using the TTFEB anion receptor in 0.5 M LiBF4, 8:2 PC/DME electrolyte and discharged at progressively lower temperatures at a C/5 rate. Even at −60°C, smooth discharges were observed and a specific capacity of nearly 275 mAh/g was obtained. In all cases, those cells made with the anion-receptor additive did not exhibit any noticeable voltage delay effects, even without the execution of a roomtemperature predischarge step. There was, instead, a characteristic positive voltage excursion upon discharge. Discussion A decrease in the electrolyte salt content from 1 to 0.5 M in an 80:20 v/v % DME/PC solution has further enhanced the lowtemperature performance of the Li/CFx electrochemical couple compared to previously published results. This improvement can be attributed to one of several mechanisms, including enhanced lowtemperature electrolyte conductivity,9 an improvement in the lowtemperature electrolyte viscosity, or a relative decrease in surface precipitation on the active cathode material surfaces when the cells are fabricated. There is not as yet conclusive proof as to which of these mechanisms 共if any兲 are at work, and this effect bears further examination. The impedance spectroscopy data indicate, however, that there is not a substantial difference between the electrode impedance as a function of salt content, which in turn indicates that the enhancement mechanism is not directly related to the ohmic losses associated with an electrode surface layer. The real impedance axis intercept is under 20 ⍀ for all cells and does not change significantly after discharge, showing that the bulk electrolyte has similar conductivity at −40°C for the three different blends examined. The A169 cathode impedance is substantially reduced after discharge, in solutions with either 0.5 or 1.0 M salt concentration, with or without the anion-receptor additive. Furthermore, previous results on threeelectrode cells indicate that much of the change in series resistance occurs on the cathode side of the cell under these conditions.2 Even though the series resistance, reflected in the x-axis intercept at high frequencies, does not change, the low-frequency impedance is significantly reduced after discharge. This may be due to inadequate wetting of the interface before discharge 共an effect that would be related to electrolyte viscosity兲 or could be due to the insulating nature of a native film that forms on the cathode before discharge. The fact that a room-temperature predischarge is not required using the lower salt content electrolyte blend can be attributed to one of several possible mechanisms. In the first, it is assumed that some portion of the electrolyte salt reacts with the cathode material upon contact to form interfacial film that impedes the cathodic reaction in some way, particularly at discharge commencement. Lowering the salt content may result in a less robust cathode surface film, because a lower salt concentration lowers the chemical driving force responsible for the formation of any interfacial layer between a CF surface and the Li-ion-containing electrolyte. A thinner cathode surface film may subsequently reduce or negate the need for a predischarge step. It is also possible that lowering the salt content results in an electrolyte with a more favorable viscosity at −40°C, as has been shown elsewhere.9 The lowered viscosity allows for a more uniform wetting of the cathode surface as well as for a more robust discharge current without polarization. It is not known if either 共or a combination兲 of these mechanisms are responsible for the observed effects. The fact that the addition of an anion receptor, tris共2,2,2trifluoroethyl borate兲, known to dissolve LiF, results in a further performance enhancement is consistent with the idea that solvating a surface LiF film on the cathode enhances performance. In intermediate cases 共i.e., C/10 or higher rates, or around 50 m in thickness兲, a substantial voltage delay was observed for cells without any anion receptor, such as that for the 57 m thick CF0.65 cathode discharged at a C/5 rate at −40°C 共Fig. 4兲. In this case, the voltage delay lasted about half of the discharge, though eventually the cell became fully functional, albeit slightly polarized. This reproducible voltage delay behavior was not observed in any of the anionreceptor-containing cells, even when discharged at a C/2.5 rate or at temperatures colder than −40°C. These observations 共when combined with the EIS results that indicate large fluctuations of the cathode impedance before and after discharge兲 are consistent with the idea that the voltage delay observed in the Li–CFx couple is related to a cathode surface film that is only partially affected when using the predischarge step. The anion receptor apparently mitigates all of the negative affects of this layer and may do so by dissolving some of the interfacial layer assumed to primarily be comprised of LiF, thereby allowing high-rate discharge at relatively cold temperatures without catastrophic cell polarization. The type of graphitic precursor used did not have a significant impact on test cell performance at low temperatures. The data in Fig. 6 indicate a roughly linear relationship between degree of fluorination and capacity, and there did not appear to be a strong correlation showing that either the graphitic or the MWNT materials offered more favorable low-temperature performance. This result is not entirely unexpected, as X-ray diffraction and electron microscopy results indicate a similar microstructure in these two types of subfluorinated carbons.3 The degree of fluorination was the strongest indicator of energy density, even at low temperatures. Because the baseline CF1.08 delivered much lower capacity 共less than 300 mAh/g兲 under these same conditions, there must be a point between x = 0.82 and 1.08 where the low-temperature efficacy of this cathode is substantially reduced, even when implemented with the better-performing electrolyte blend and anion receptor identified in this work. A170 Electrochemical and Solid-State Letters, 10 共7兲 A166-A170 共2007兲 This may be attributed to enhanced low-temperature electrolyte viscosity and/or a diminished tendency to form a resistive native cathode/electrolyte SEI. Three variations of SFCFx cathode materials were inserted into similar ⬃40 m thick composite electrode structures and tested at −40°C using several different electrolyte blends. The CF0.65- and CF0.82-based cells could deliver well over 600 mAh/g above 2 V under a C/5 discharge rate at −40°C with the proper electrolyte blend. To further increase rate capability and/or functional cathode thickness, an anion-receptor electrolyte additive, TTFEB, was evaluated and proved to be effective. With this additive, composite cathode structures 115 m thick yielded over 500 mAh/g at a C/5 discharge rate at −40°C. These results indicate that the CF/electrolyte interfacial area, the viscosity of the electrolyte, and the nature of any surface film that may form on these active areas are critical to low-temperature performance. The modifications implemented resulted in a greatly enhanced low-temperature performance for this useful electrochemical couple and have enabled cells that are functional to temperatures −60°C and possibly colder. Acknowledgments The work described here was carried out at the Jet Propulsion Laboratory, California Institute of Technology, for the NASA ESMD technology development program, under contract with the National Aeronautics and Space Administration 共NASA兲. Figure 6. 共Color online兲 Capacity yielded at −40°C from SFCFx test cells based on either graphitic 共GII兲 or MWNT 共GIII兲 precursor material. A C/10 discharge was used in all cases, and all cells were approximately 40 m in thickness. Conclusion The results are consistent with previously published suggestions that the nanoscale intermixing of pristine graphitic domains and partially fluorinated domains observed in SFCFx materials greatly enhance the specific capacity of these materials at low temperatures at aggressive rates.2 Electrolyte screening identified that blends consisting of 20:80 v/v % PC/DME with 0.5 M LiBF4 offered superior low-temperature performance compared to the baseline formulations, based on 1 M LiBF4 in either 50:50 or 20:80 v/v % PC/DME. California Institute of Technology assisted in meeting the publication costs of this article. References 1. P. Lam and R. Yazami, J. Power Sources, 153, 354 共2006兲. 2. J. F. Whitacre, R. Yazami, and A. Hamwi, M. C. Smart, W. Bennett, G. K. S. Prakash, T. Miller, and R. V. Bugga, J. Power Sources, 160, 577 共2006兲. 3. K. Guerin, R. Yazami, and A. Hamwi, Electrochem. Solid-State Lett., 7, A159 共2004兲. 4. H. S. Lee et al., J. Electrochem. Soc., 151, A1429 共2004兲. 5. X. H. Sun et al., Electrochem. Solid-State Lett., 6, A43 共2003兲. 6. X. Sun et al., Electrochem. Solid-State Lett., 1, 239 共1998兲. 7. T. I. M. Fukuda and T. Iijima, in Fifth Power Sources Conference, D. H. Collins, Editor, Academic, New York 共1975兲, p. 713. 8. R. G. Gunther, in Fifth Power Sources Conference, D. H. Collins, Editor, Academic, New York 共1975兲, p. 729. 9. M. S. Ding, K. Xu, S. S. Zhang, K. Amine, G. L. Henriksen, and T. R. Jow, J. Electrochem. Soc., 148, A1196 共2001兲.